#------------------------------------------------------------------------------
#$Date: 2016-03-25 11:31:19 +0200 (Fri, 25 Mar 2016) $
#$Revision: 179794 $
#$URL: svn://www.crystallography.net/cod/cif/7/00/90/7009007.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7009007
loop_
_publ_author_name
'Paul M. O'Meara'
'Marten G. Barker'
'Alexander J. Blake'
'Paul A. Cooke'
'Duncan H. Gregory'
_publ_section_title
;
 Synthesis and crystal structure of a new strontium nitridomolybdate
 oxide, Sr4[MoN4]O
;
_journal_issue                   5
_journal_name_full               'J. Chem. Soc., Dalton Trans.'
_journal_page_first              633
_journal_page_last               638
_journal_paper_doi               10.1039/a907843f
_journal_year                    2000
_chemical_formula_moiety         'Sr4 Mo N4 O'
_chemical_formula_sum            'Mo N4 O Sr4'
_chemical_formula_weight         518.46
_chemical_name_common            'strontium nitridomolybdate oxide'
_chemical_name_systematic
;
tetra strontium oxonitridomolybdate (VI)
;
_space_group_IT_number           11
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 102.08(7)
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   8.951(11)
_cell_length_b                   14.694(12)
_cell_length_c                   10.715(10)
_cell_measurement_reflns_used    30
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      17.4
_cell_measurement_theta_min      13
_cell_volume                     1378(2)
_computing_cell_refinement       'STADI4 (STOE, 1996)'
_computing_data_collection       'STADI4 (STOE, 1996)'
_computing_data_reduction        'X-RED (STOE, 1996)'
_computing_molecular_graphics    'ATOMS 4.1 (Dowty, 1998)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SIR97 (Giacovazzo, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device_type  'STOE STADI4 4-circle-diffractometer D092'
_diffrn_measurement_method
;
 'tetra strontium oxonitridomolybdate (VI)'
;
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0665
_diffrn_reflns_av_sigmaI/netI    0.0487
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            3575
_diffrn_reflns_theta_full        25.01
_diffrn_reflns_theta_max         25.01
_diffrn_reflns_theta_min         2.70
_diffrn_standards_decay_%        5.3
_diffrn_standards_interval_time  60
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    32.457
_exptl_absorpt_correction_T_max  0.514
_exptl_absorpt_correction_T_min  0.07
_exptl_absorpt_correction_type   refdelf
_exptl_absorpt_process_details
;
 'tetra strontium oxonitridomolybdate (VI)'
;
_exptl_crystal_colour            'dark blue'
_exptl_crystal_density_diffrn    4.998
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    .
_exptl_crystal_description       'rectangular block'
_exptl_crystal_F_000             1840
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.263
_exptl_crystal_size_min          0.13
_refine_diff_density_max         2.330
_refine_diff_density_min         -1.847
_refine_diff_density_rms         0.314
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.057
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     199
_refine_ls_number_reflns         2532
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.057
_refine_ls_R_factor_all          0.0671
_refine_ls_R_factor_gt           0.0480
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0678P)²+9.1933P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1175
_refine_ls_wR_factor_ref         0.1303
_reflns_number_gt                1963
_reflns_number_total             2532
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            a907843f.txt
_cod_data_source_block           srmon42
_cod_original_sg_symbol_H-M      'P 2 1/m'
_cod_database_code               7009007
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'
'-x, -y, -z'
'x, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.89292(19) -0.2500 0.96495(14) 0.0209(4) Uani 1 2 d S . .
Mo2 Mo 0.57108(13) -0.01623(7) 0.25210(10) 0.0213(3) Uani 1 1 d . . .
Mo3 Mo 0.9356(2) 0.2500 0.51786(15) 0.0244(4) Uani 1 2 d S . .
Sr1 Sr 0.4095(2) -0.2500 0.69702(17) 0.0292(5) Uani 1 2 d S . .
Sr2 Sr 0.5970(2) -0.2500 0.31288(16) 0.0227(4) Uani 1 2 d S . .
Sr3 Sr 1.11302(14) -0.12767(8) 0.80253(11) 0.0222(3) Uani 1 1 d . . .
Sr4 Sr 0.66956(15) 0.10504(8) 0.56611(11) 0.0257(3) Uani 1 1 d . . .
Sr5 Sr 0.7612(2) 0.2500 0.87577(15) 0.0210(4) Uani 1 2 d S . .
Sr6 Sr 0.20039(14) 0.00247(8) 0.10548(11) 0.0214(3) Uani 1 1 d . . .
Sr7 Sr 1.0000 0.0000 0.5000 0.0300(4) Uani 1 2 d S . .
Sr8 Sr 0.48535(15) 0.13037(8) 0.01579(11) 0.0215(3) Uani 1 1 d . . .
Sr9 Sr 1.09401(14) 0.12569(8) 0.77382(11) 0.0223(3) Uani 1 1 d . . .
Sr10 Sr 0.73893(15) -0.13931(8) 0.60784(11) 0.0247(3) Uani 1 1 d . . .
N1 N 0.8578(17) 0.2500 0.6668(14) 0.020(3) Uani 1 2 d S . .
N2 N 0.858(2) -0.2500 0.7874(13) 0.026(4) Uani 1 2 d S . .
N3 N 0.4500(14) 0.0877(8) 0.2505(10) 0.027(3) Uani 1 1 d . . .
N4 N 1.3128(12) 0.0053(6) 0.8757(10) 0.021(2) Uani 1 1 d . . .
N5 N 0.6893(16) -0.0448(9) 0.4067(11) 0.041(3) Uani 1 1 d . . .
N6 N 0.5734(13) 0.1117(7) -0.2010(10) 0.023(2) Uani 1 1 d . . .
N7 N 1.0131(13) -0.1440(7) 1.0192(10) 0.024(2) Uani 1 1 d . . .
N8 N 0.738(2) -0.2500 1.0596(14) 0.030(4) Uani 1 2 d S . .
N9 N 0.8530(18) 0.1508(9) 0.4232(11) 0.048(4) Uani 1 1 d . . .
N10 N 0.854(2) -0.2500 0.436(2) 0.051(5) Uani 1 2 d S . .
O1 O 0.9115(10) -0.0045(6) 0.7061(8) 0.024(2) Uani 1 1 d . . .
O2 O 0.5153(17) -0.2500 0.5095(13) 0.031(3) Uani 1 2 d S . .
O3 O 0.6811(16) 0.2500 1.0950(12) 0.025(3) Uani 1 2 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N2 Mo1 N8 124.4(7) . . ?
N2 Mo1 N7 105.9(4) . . ?
N8 Mo1 N7 105.5(4) . . ?
N2 Mo1 N7 105.9(4) . 4 ?
N8 Mo1 N7 105.5(4) . 4 ?
N7 Mo1 N7 109.0(6) . 4 ?
N2 Mo1 Sr5 118.7(6) . 3_757 ?
N8 Mo1 Sr5 116.9(5) . 3_757 ?
N7 Mo1 Sr5 54.5(3) . 3_757 ?
N7 Mo1 Sr5 54.5(3) 4 3_757 ?
N2 Mo1 Sr9 146.01(11) . 3_757 ?
N8 Mo1 Sr9 56.4(4) . 3_757 ?
N7 Mo1 Sr9 51.6(3) . 3_757 ?
N7 Mo1 Sr9 105.8(3) 4 3_757 ?
Sr5 Mo1 Sr9 72.06(7) 3_757 3_757 ?
N2 Mo1 Sr9 146.01(11) . 2_747 ?
N8 Mo1 Sr9 56.4(4) . 2_747 ?
N7 Mo1 Sr9 105.8(3) . 2_747 ?
N7 Mo1 Sr9 51.6(3) 4 2_747 ?
Sr5 Mo1 Sr9 72.06(7) 3_757 2_747 ?
Sr9 Mo1 Sr9 66.67(8) 3_757 2_747 ?
N2 Mo1 Sr3 57.9(4) . . ?
N8 Mo1 Sr3 147.85(8) . . ?
N7 Mo1 Sr3 51.4(3) . . ?
N7 Mo1 Sr3 103.7(3) 4 . ?
Sr5 Mo1 Sr3 71.00(8) 3_757 . ?
Sr9 Mo1 Sr3 102.61(7) 3_757 . ?
Sr9 Mo1 Sr3 143.03(8) 2_747 . ?
N2 Mo1 Sr3 57.9(4) . 4 ?
N8 Mo1 Sr3 147.85(8) . 4 ?
N7 Mo1 Sr3 103.7(3) . 4 ?
N7 Mo1 Sr3 51.4(3) 4 4 ?
Sr5 Mo1 Sr3 71.00(8) 3_757 4 ?
Sr9 Mo1 Sr3 143.03(7) 3_757 4 ?
Sr9 Mo1 Sr3 102.61(7) 2_747 4 ?
Sr3 Mo1 Sr3 63.78(8) . 4 ?
N2 Mo1 Sr6 79.22(11) . 2_646 ?
N8 Mo1 Sr6 87.15(14) . 2_646 ?
N7 Mo1 Sr6 158.8(3) . 2_646 ?
N7 Mo1 Sr6 50.4(3) 4 2_646 ?
Sr5 Mo1 Sr6 104.78(4) 3_757 2_646 ?
Sr9 Mo1 Sr6 131.73(5) 3_757 2_646 ?
Sr9 Mo1 Sr6 66.79(6) 2_747 2_646 ?
Sr3 Mo1 Sr6 122.32(6) . 2_646 ?
Sr3 Mo1 Sr6 61.05(5) 4 2_646 ?
N2 Mo1 Sr6 79.22(11) . 3_656 ?
N8 Mo1 Sr6 87.15(14) . 3_656 ?
N7 Mo1 Sr6 50.4(3) . 3_656 ?
N7 Mo1 Sr6 158.8(3) 4 3_656 ?
Sr5 Mo1 Sr6 104.78(4) 3_757 3_656 ?
Sr9 Mo1 Sr6 66.79(6) 3_757 3_656 ?
Sr9 Mo1 Sr6 131.73(5) 2_747 3_656 ?
Sr3 Mo1 Sr6 61.05(5) . 3_656 ?
Sr3 Mo1 Sr6 122.32(6) 4 3_656 ?
Sr6 Mo1 Sr6 149.20(7) 2_646 3_656 ?
N2 Mo1 Sr8 95.4(5) . 2_646 ?
N8 Mo1 Sr8 38.5(3) . 2_646 ?
N7 Mo1 Sr8 143.0(3) . 2_646 ?
N7 Mo1 Sr8 93.3(3) 4 2_646 ?
Sr5 Mo1 Sr8 137.03(7) 3_757 2_646 ?
Sr9 Mo1 Sr8 94.70(8) 3_757 2_646 ?
Sr9 Mo1 Sr8 65.25(7) 2_747 2_646 ?
Sr3 Mo1 Sr8 151.22(6) . 2_646 ?
Sr3 Mo1 Sr8 113.28(7) 4 2_646 ?
Sr6 Mo1 Sr8 53.95(4) 2_646 2_646 ?
Sr6 Mo1 Sr8 106.85(7) 3_656 2_646 ?
N5 Mo2 N3 115.0(5) . . ?
N5 Mo2 N4 112.1(6) . 3_756 ?
N3 Mo2 N4 109.2(4) . 3_756 ?
N5 Mo2 N6 108.8(5) . 3_655 ?
N3 Mo2 N6 103.9(5) . 3_655 ?
N4 Mo2 N6 107.3(4) 3_756 3_655 ?
N5 Mo2 Sr8 129.4(4) . 3_655 ?
N3 Mo2 Sr8 115.3(3) . 3_655 ?
N4 Mo2 Sr8 54.2(3) 3_756 3_655 ?
N6 Mo2 Sr8 53.2(3) 3_655 3_655 ?
N5 Mo2 Sr8 148.2(4) . . ?
N3 Mo2 Sr8 54.3(3) . . ?
N4 Mo2 Sr8 57.5(3) 3_756 . ?
N6 Mo2 Sr8 103.0(3) 3_655 . ?
Sr8 Mo2 Sr8 72.07(8) 3_655 . ?
N5 Mo2 Sr6 140.5(5) . . ?
N3 Mo2 Sr6 54.4(4) . . ?
N4 Mo2 Sr6 107.0(3) 3_756 . ?
N6 Mo2 Sr6 52.0(3) 3_655 . ?
Sr8 Mo2 Sr6 71.14(7) 3_655 . ?
Sr8 Mo2 Sr6 62.61(6) . . ?
N5 Mo2 Sr4 73.2(5) . 3_656 ?
N3 Mo2 Sr4 83.4(4) . 3_656 ?
N4 Mo2 Sr4 160.7(3) 3_756 3_656 ?
N6 Mo2 Sr4 54.4(3) 3_655 3_656 ?
Sr8 Mo2 Sr4 107.55(7) 3_655 3_656 ?
Sr8 Mo2 Sr4 127.57(7) . 3_656 ?
Sr6 Mo2 Sr4 67.91(8) . 3_656 ?
N5 Mo2 Sr9 67.5(5) . 3_756 ?
N3 Mo2 Sr9 152.6(4) . 3_756 ?
N4 Mo2 Sr9 50.6(3) 3_756 3_756 ?
N6 Mo2 Sr9 100.5(3) 3_655 3_756 ?
Sr8 Mo2 Sr9 70.66(7) 3_655 3_756 ?
Sr8 Mo2 Sr9 107.98(7) . 3_756 ?
Sr6 Mo2 Sr9 141.64(6) . 3_756 ?
Sr4 Mo2 Sr9 121.53(7) 3_656 3_756 ?
N5 Mo2 Sr2 66.4(4) . . ?
N3 Mo2 Sr2 145.1(4) . . ?
N4 Mo2 Sr2 101.1(3) 3_756 . ?
N6 Mo2 Sr2 49.1(3) 3_655 . ?
Sr8 Mo2 Sr2 69.61(6) 3_655 . ?
Sr8 Mo2 Sr2 141.49(5) . . ?
Sr6 Mo2 Sr2 100.80(5) . . ?
Sr4 Mo2 Sr2 63.11(5) 3_656 . ?
Sr9 Mo2 Sr2 62.21(5) 3_756 . ?
N5 Mo2 Sr3 87.6(5) . 3_756 ?
N3 Mo2 Sr3 89.6(4) . 3_756 ?
N4 Mo2 Sr3 43.8(3) 3_756 3_756 ?
N6 Mo2 Sr3 151.0(3) 3_655 3_756 ?
Sr8 Mo2 Sr3 97.93(7) 3_655 3_756 ?
Sr8 Mo2 Sr3 64.15(7) . 3_756 ?
Sr6 Mo2 Sr3 126.43(7) . 3_756 ?
Sr4 Mo2 Sr3 154.18(5) 3_656 3_756 ?
Sr9 Mo2 Sr3 63.05(8) 3_756 3_756 ?
Sr2 Mo2 Sr3 124.89(7) . 3_756 ?
N5 Mo2 Sr4 46.3(4) . . ?
N3 Mo2 Sr4 69.3(3) . . ?
N4 Mo2 Sr4 123.2(3) 3_756 . ?
N6 Mo2 Sr4 128.7(3) 3_655 . ?
Sr8 Mo2 Sr4 174.99(5) 3_655 . ?
Sr8 Mo2 Sr4 110.66(8) . . ?
Sr6 Mo2 Sr4 113.79(7) . . ?
Sr4 Mo2 Sr4 74.34(7) 3_656 . ?
Sr9 Mo2 Sr4 104.36(8) 3_756 . ?
Sr2 Mo2 Sr4 107.83(6) . . ?
Sr3 Mo2 Sr4 79.92(7) 3_756 . ?
N9 Mo3 N9 104.8(9) . 4_565 ?
N9 Mo3 N10 114.7(6) . 3_756 ?
N9 Mo3 N10 114.7(6) 4_565 3_756 ?
N9 Mo3 N1 107.0(5) . . ?
N9 Mo3 N1 107.0(5) 4_565 . ?
N10 Mo3 N1 108.3(8) 3_756 . ?
N9 Mo3 Sr4 50.1(4) . . ?
N9 Mo3 Sr4 112.1(5) 4_565 . ?
N10 Mo3 Sr4 133.2(3) 3_756 . ?
N1 Mo3 Sr4 57.3(3) . . ?
N9 Mo3 Sr4 112.1(5) . 4_565 ?
N9 Mo3 Sr4 50.1(4) 4_565 4_565 ?
N10 Mo3 Sr4 133.2(3) 3_756 4_565 ?
N1 Mo3 Sr4 57.3(3) . 4_565 ?
Sr4 Mo3 Sr4 79.96(10) . 4_565 ?
N9 Mo3 Sr9 159.2(4) . 4_565 ?
N9 Mo3 Sr9 94.1(4) 4_565 4_565 ?
N10 Mo3 Sr9 63.1(5) 3_756 4_565 ?
N1 Mo3 Sr9 58.1(4) . 4_565 ?
Sr4 Mo3 Sr9 114.65(8) . 4_565 ?
Sr4 Mo3 Sr9 73.56(8) 4_565 4_565 ?
N9 Mo3 Sr9 94.1(4) . . ?
N9 Mo3 Sr9 159.2(4) 4_565 . ?
N10 Mo3 Sr9 63.1(5) 3_756 . ?
N1 Mo3 Sr9 58.1(4) . . ?
Sr4 Mo3 Sr9 73.56(8) . . ?
Sr4 Mo3 Sr9 114.65(8) 4_565 . ?
Sr9 Mo3 Sr9 66.02(8) 4_565 . ?
N9 Mo3 Sr1 55.3(5) . 3_656 ?
N9 Mo3 Sr1 55.3(5) 4_565 3_656 ?
N10 Mo3 Sr1 154.3(7) 3_756 3_656 ?
N1 Mo3 Sr1 97.4(5) . 3_656 ?
Sr4 Mo3 Sr1 62.06(7) . 3_656 ?
Sr4 Mo3 Sr1 62.06(7) 4_565 3_656 ?
Sr9 Mo3 Sr1 135.51(6) 4_565 3_656 ?
Sr9 Mo3 Sr1 135.51(6) . 3_656 ?
N9 Mo3 Sr7 143.2(4) . 2_756 ?
N9 Mo3 Sr7 40.5(5) 4_565 2_756 ?
N10 Mo3 Sr7 81.57(7) 3_756 2_756 ?
N1 Mo3 Sr7 97.64(6) . 2_756 ?
Sr4 Mo3 Sr7 139.88(6) . 2_756 ?
Sr4 Mo3 Sr7 59.93(6) 4_565 2_756 ?
Sr9 Mo3 Sr7 57.45(4) 4_565 2_756 ?
Sr9 Mo3 Sr7 122.35(6) . 2_756 ?
Sr1 Mo3 Sr7 95.30(3) 3_656 2_756 ?
N9 Mo3 Sr7 40.5(5) . . ?
N9 Mo3 Sr7 143.2(4) 4_565 . ?
N10 Mo3 Sr7 81.57(7) 3_756 . ?
N1 Mo3 Sr7 97.64(6) . . ?
Sr4 Mo3 Sr7 59.93(6) . . ?
Sr4 Mo3 Sr7 139.88(6) 4_565 . ?
Sr9 Mo3 Sr7 122.35(6) 4_565 . ?
Sr9 Mo3 Sr7 57.45(4) . . ?
Sr1 Mo3 Sr7 95.30(3) 3_656 . ?
Sr7 Mo3 Sr7 160.10(6) 2_756 . ?
N9 Mo3 Sr3 34.4(4) . 3_756 ?
N9 Mo3 Sr3 85.4(4) 4_565 3_756 ?
N10 Mo3 Sr3 99.1(6) 3_756 3_756 ?
N1 Mo3 Sr3 140.8(3) . 3_756 ?
Sr4 Mo3 Sr3 83.53(7) . 3_756 ?
Sr4 Mo3 Sr3 119.49(8) 4_565 3_756 ?
Sr9 Mo3 Sr3 160.22(7) 4_565 3_756 ?
Sr9 Mo3 Sr3 115.34(7) . 3_756 ?
Sr1 Mo3 Sr3 58.77(7) 3_656 3_756 ?
Sr7 Mo3 Sr3 114.03(5) 2_756 3_756 ?
Sr7 Mo3 Sr3 58.66(4) . 3_756 ?
O2 Sr1 O3 175.5(5) . 3_657 ?
O2 Sr1 N3 85.8(3) . 3_656 ?
O3 Sr1 N3 92.2(3) 3_657 3_656 ?
O2 Sr1 N3 85.8(3) . 2_646 ?
O3 Sr1 N3 92.2(3) 3_657 2_646 ?
N3 Sr1 N3 124.1(5) 3_656 2_646 ?
O2 Sr1 N9 93.1(4) . 2_646 ?
O3 Sr1 N9 90.7(4) 3_657 2_646 ?
N3 Sr1 N9 148.7(4) 3_656 2_646 ?
N3 Sr1 N9 86.9(4) 2_646 2_646 ?
O2 Sr1 N9 93.1(4) . 3_656 ?
O3 Sr1 N9 90.7(4) 3_657 3_656 ?
N3 Sr1 N9 86.9(4) 3_656 3_656 ?
N3 Sr1 N9 148.7(4) 2_646 3_656 ?
N9 Sr1 N9 61.9(6) 2_646 3_656 ?
O2 Sr1 Mo3 84.0(4) . 3_656 ?
O3 Sr1 Mo3 100.4(3) 3_657 3_656 ?
N3 Sr1 Mo3 116.9(2) 3_656 3_656 ?
N3 Sr1 Mo3 116.9(2) 2_646 3_656 ?
N9 Sr1 Mo3 32.3(3) 2_646 3_656 ?
N9 Sr1 Mo3 32.3(3) 3_656 3_656 ?
O2 Sr1 Sr4 51.0(2) . 2_646 ?
O3 Sr1 Sr4 131.7(2) 3_657 2_646 ?
N3 Sr1 Sr4 135.6(2) 3_656 2_646 ?
N3 Sr1 Sr4 68.6(2) 2_646 2_646 ?
N9 Sr1 Sr4 46.3(3) 2_646 2_646 ?
N9 Sr1 Sr4 86.4(3) 3_656 2_646 ?
Mo3 Sr1 Sr4 57.15(6) 3_656 2_646 ?
O2 Sr1 Sr4 51.0(2) . 3_656 ?
O3 Sr1 Sr4 131.7(2) 3_657 3_656 ?
N3 Sr1 Sr4 68.6(2) 3_656 3_656 ?
N3 Sr1 Sr4 135.6(2) 2_646 3_656 ?
N9 Sr1 Sr4 86.4(3) 2_646 3_656 ?
N9 Sr1 Sr4 46.3(3) 3_656 3_656 ?
Mo3 Sr1 Sr4 57.15(6) 3_656 3_656 ?
Sr4 Sr1 Sr4 75.33(9) 2_646 3_656 ?
O2 Sr1 Sr8 131.1(3) . 3_656 ?
O3 Sr1 Sr8 45.6(2) 3_657 3_656 ?
N3 Sr1 Sr8 49.1(2) 3_656 3_656 ?
N3 Sr1 Sr8 103.5(2) 2_646 3_656 ?
N9 Sr1 Sr8 134.7(3) 2_646 3_656 ?
N9 Sr1 Sr8 100.7(3) 3_656 3_656 ?
Mo3 Sr1 Sr8 128.81(7) 3_656 3_656 ?
Sr4 Sr1 Sr8 172.05(5) 2_646 3_656 ?
Sr4 Sr1 Sr8 112.10(7) 3_656 3_656 ?
O2 Sr1 Sr8 131.1(3) . 2_646 ?
O3 Sr1 Sr8 45.6(2) 3_657 2_646 ?
N3 Sr1 Sr8 103.5(2) 3_656 2_646 ?
N3 Sr1 Sr8 49.1(2) 2_646 2_646 ?
N9 Sr1 Sr8 100.7(3) 2_646 2_646 ?
N9 Sr1 Sr8 134.7(3) 3_656 2_646 ?
Mo3 Sr1 Sr8 128.81(7) 3_656 2_646 ?
Sr4 Sr1 Sr8 112.10(7) 2_646 2_646 ?
Sr4 Sr1 Sr8 172.05(5) 3_656 2_646 ?
Sr8 Sr1 Sr8 60.34(8) 3_656 2_646 ?
O2 Sr1 Sr3 135.6(2) . 4_455 ?
O3 Sr1 Sr3 47.6(2) 3_657 4_455 ?
N3 Sr1 Sr3 136.2(2) 3_656 4_455 ?
N3 Sr1 Sr3 80.5(3) 2_646 4_455 ?
N9 Sr1 Sr3 44.5(3) 2_646 4_455 ?
N9 Sr1 Sr3 78.6(3) 3_656 4_455 ?
Mo3 Sr1 Sr3 65.84(8) 3_656 4_455 ?
Sr4 Sr1 Sr3 84.85(7) 2_646 4_455 ?
Sr4 Sr1 Sr3 121.60(9) 3_656 4_455 ?
Sr8 Sr1 Sr3 93.17(8) 3_656 4_455 ?
Sr8 Sr1 Sr3 63.29(8) 2_646 4_455 ?
O2 Sr2 N10 87.1(6) . . ?
O2 Sr2 N6 98.4(3) . 2_645 ?
N10 Sr2 N6 129.7(3) . 2_645 ?
O2 Sr2 N6 98.4(3) . 3_655 ?
N10 Sr2 N6 129.7(3) . 3_655 ?
N6 Sr2 N6 99.1(5) 2_645 3_655 ?
O2 Sr2 N8 175.1(5) . 1_554 ?
N10 Sr2 N8 88.0(6) . 1_554 ?
N6 Sr2 N8 84.8(3) 2_645 1_554 ?
N6 Sr2 N8 84.8(3) 3_655 1_554 ?
O2 Sr2 N5 80.2(3) . . ?
N10 Sr2 N5 71.1(2) . . ?
N6 Sr2 N5 159.2(3) 2_645 . ?
N6 Sr2 N5 60.9(3) 3_655 . ?
N8 Sr2 N5 98.2(3) 1_554 . ?
O2 Sr2 N5 80.2(3) . 4 ?
N10 Sr2 N5 71.1(2) . 4 ?
N6 Sr2 N5 60.9(3) 2_645 4 ?
N6 Sr2 N5 159.2(3) 3_655 4 ?
N8 Sr2 N5 98.2(3) 1_554 4 ?
N5 Sr2 N5 137.9(4) . 4 ?
O2 Sr2 Sr5 95.7(4) . 3_656 ?
N10 Sr2 Sr5 177.2(5) . 3_656 ?
N6 Sr2 Sr5 50.0(2) 2_645 3_656 ?
N6 Sr2 Sr5 50.0(2) 3_655 3_656 ?
N8 Sr2 Sr5 89.2(3) 1_554 3_656 ?
N5 Sr2 Sr5 109.4(2) . 3_656 ?
N5 Sr2 Sr5 109.4(2) 4 3_656 ?
O2 Sr2 Mo2 98.33(5) . 4 ?
N10 Sr2 Mo2 96.95(8) . 4 ?
N6 Sr2 Mo2 32.7(2) 2_645 4 ?
N6 Sr2 Mo2 130.9(2) 3_655 4 ?
N8 Sr2 Mo2 82.27(5) 1_554 4 ?
N5 Sr2 Mo2 168.0(2) . 4 ?
N5 Sr2 Mo2 31.05(19) 4 4 ?
Sr5 Sr2 Mo2 82.66(4) 3_656 4 ?
O2 Sr2 Mo2 98.33(5) . . ?
N10 Sr2 Mo2 96.95(8) . . ?
N6 Sr2 Mo2 130.9(2) 2_645 . ?
N6 Sr2 Mo2 32.7(2) 3_655 . ?
N8 Sr2 Mo2 82.27(5) 1_554 . ?
N5 Sr2 Mo2 31.05(19) . . ?
N5 Sr2 Mo2 168.0(2) 4 . ?
Sr5 Sr2 Mo2 82.66(4) 3_656 . ?
Mo2 Sr2 Mo2 158.76(7) 4 . ?
O2 Sr2 Sr10 47.7(3) . . ?
N10 Sr2 Sr10 52.1(4) . . ?
N6 Sr2 Sr10 144.5(2) 2_645 . ?
N6 Sr2 Sr10 96.6(2) 3_655 . ?
N8 Sr2 Sr10 128.4(3) 1_554 . ?
N5 Sr2 Sr10 43.4(2) . . ?
N5 Sr2 Sr10 97.5(2) 4 . ?
Sr5 Sr2 Sr10 130.16(7) 3_656 . ?
Mo2 Sr2 Sr10 127.91(5) 4 . ?
Mo2 Sr2 Sr10 73.30(5) . . ?
O2 Sr2 Sr10 47.7(3) . 4 ?
N10 Sr2 Sr10 52.1(4) . 4 ?
N6 Sr2 Sr10 96.6(2) 2_645 4 ?
N6 Sr2 Sr10 144.5(2) 3_655 4 ?
N8 Sr2 Sr10 128.4(3) 1_554 4 ?
N5 Sr2 Sr10 97.5(2) . 4 ?
N5 Sr2 Sr10 43.4(2) 4 4 ?
Sr5 Sr2 Sr10 130.16(7) 3_656 4 ?
Mo2 Sr2 Sr10 73.30(5) 4 4 ?
Mo2 Sr2 Sr10 127.91(5) . 4 ?
Sr10 Sr2 Sr10 54.62(8) . 4 ?
N9 Sr3 O1 85.8(4) 3_756 . ?
N9 Sr3 O3 95.3(4) 3_756 3_757 ?
O1 Sr3 O3 178.7(3) . 3_757 ?
N9 Sr3 N4 100.0(4) 3_756 . ?
O1 Sr3 N4 88.5(3) . . ?
O3 Sr3 N4 90.6(3) 3_757 . ?
N9 Sr3 N7 162.1(4) 3_756 . ?
O1 Sr3 N7 94.4(3) . . ?
O3 Sr3 N7 84.8(4) 3_757 . ?
N4 Sr3 N7 97.9(3) . . ?
N9 Sr3 N2 96.6(4) 3_756 . ?
O1 Sr3 N2 86.4(3) . . ?
O3 Sr3 N2 94.3(3) 3_757 . ?
N4 Sr3 N2 162.2(4) . . ?
N7 Sr3 N2 65.6(4) . . ?
N9 Sr3 Mo1 128.2(3) 3_756 . ?
O1 Sr3 Mo1 98.2(2) . . ?
O3 Sr3 Mo1 81.7(3) 3_757 . ?
N4 Sr3 Mo1 131.6(2) . . ?
N7 Sr3 Mo1 34.1(2) . . ?
N2 Sr3 Mo1 33.2(3) . . ?
N9 Sr3 Sr10 73.7(4) 3_756 . ?
O1 Sr3 Sr10 46.7(2) . . ?
O3 Sr3 Sr10 134.4(2) 3_757 . ?
N4 Sr3 Sr10 134.5(2) . . ?
N7 Sr3 Sr10 93.5(2) . . ?
N2 Sr3 Sr10 45.6(3) . . ?
Mo1 Sr3 Sr10 72.54(8) . . ?
N9 Sr3 Sr1 51.9(4) 3_756 1_655 ?
O1 Sr3 Sr1 136.0(2) . 1_655 ?
O3 Sr3 Sr1 44.8(3) 3_757 1_655 ?
N4 Sr3 Sr1 88.0(2) . 1_655 ?
N7 Sr3 Sr1 129.4(2) . 1_655 ?
N2 Sr3 Sr1 107.4(2) . 1_655 ?
Mo1 Sr3 Sr1 116.31(8) . 1_655 ?
Sr10 Sr3 Sr1 117.36(8) . 1_655 ?
N9 Sr3 Sr3 82.3(3) 3_756 4 ?
O1 Sr3 Sr3 133.9(2) . 4 ?
O3 Sr3 Sr3 47.2(2) 3_757 4 ?
N4 Sr3 Sr3 137.4(2) . 4 ?
N7 Sr3 Sr3 84.8(2) . 4 ?
N2 Sr3 Sr3 51.4(2) . 4 ?
Mo1 Sr3 Sr3 58.11(4) . 4 ?
Sr10 Sr3 Sr3 87.25(3) . 4 ?
Sr1 Sr3 Sr3 59.85(4) 1_655 4 ?
N9 Sr3 Sr6 125.4(4) 3_756 3_656 ?
O1 Sr3 Sr6 41.6(2) . 3_656 ?
O3 Sr3 Sr6 137.5(3) 3_757 3_656 ?
N4 Sr3 Sr6 93.3(2) . 3_656 ?
N7 Sr3 Sr6 52.8(2) . 3_656 ?
N2 Sr3 Sr6 71.7(2) . 3_656 ?
Mo1 Sr3 Sr6 64.48(7) . 3_656 ?
Sr10 Sr3 Sr6 60.11(7) . 3_656 ?
Sr1 Sr3 Sr6 177.25(5) 1_655 3_656 ?
Sr3 Sr3 Sr6 120.19(4) 4 3_656 ?
N9 Sr3 Mo2 70.9(3) 3_756 3_756 ?
O1 Sr3 Mo2 91.7(2) . 3_756 ?
O3 Sr3 Mo2 88.0(3) 3_757 3_756 ?
N4 Sr3 Mo2 29.5(2) . 3_756 ?
N7 Sr3 Mo2 126.8(2) . 3_756 ?
N2 Sr3 Mo2 167.5(3) . 3_756 ?
Mo1 Sr3 Mo2 158.87(5) . 3_756 ?
Sr10 Sr3 Mo2 126.53(7) . 3_756 ?
Sr1 Sr3 Mo2 65.95(8) 1_655 3_756 ?
Sr3 Sr3 Mo2 125.13(5) 4 3_756 ?
Sr6 Sr3 Mo2 114.37(8) 3_656 3_756 ?
N9 Sr4 O2 92.4(5) . 3_656 ?
N9 Sr4 N1 67.6(4) . . ?
O2 Sr4 N1 78.3(3) 3_656 . ?
N9 Sr4 N6 151.4(4) . 1_556 ?
O2 Sr4 N6 87.5(4) 3_656 1_556 ?
N1 Sr4 N6 84.4(4) . 1_556 ?
N9 Sr4 N5 73.3(4) . . ?
O2 Sr4 N5 123.0(4) 3_656 . ?
N1 Sr4 N5 136.3(4) . . ?
N6 Sr4 N5 129.5(4) 1_556 . ?
N9 Sr4 O1 87.2(4) . . ?
O2 Sr4 O1 161.1(3) 3_656 . ?
N1 Sr4 O1 84.1(3) . . ?
N6 Sr4 O1 83.8(3) 1_556 . ?
N5 Sr4 O1 75.0(3) . . ?
N9 Sr4 Mo3 33.5(3) . . ?
O2 Sr4 Mo3 82.1(3) 3_656 . ?
N1 Sr4 Mo3 34.3(3) . . ?
N6 Sr4 Mo3 118.7(2) 1_556 . ?
N5 Sr4 Mo3 105.6(3) . . ?
O1 Sr4 Mo3 87.3(2) . . ?
N9 Sr4 Mo2 173.0(3) . 3_656 ?
O2 Sr4 Mo2 93.0(3) 3_656 3_656 ?
N1 Sr4 Mo2 118.0(3) . 3_656 ?
N6 Sr4 Mo2 33.6(2) 1_556 3_656 ?
N5 Sr4 Mo2 99.9(3) . 3_656 ?
O1 Sr4 Mo2 89.1(2) . 3_656 ?
Mo3 Sr4 Mo2 152.27(6) . 3_656 ?
N9 Sr4 Sr1 53.3(3) . 3_656 ?
O2 Sr4 Sr1 43.2(3) 3_656 3_656 ?
N1 Sr4 Sr1 81.4(3) . 3_656 ?
N6 Sr4 Sr1 130.5(2) 1_556 3_656 ?
N5 Sr4 Sr1 90.9(2) . 3_656 ?
O1 Sr4 Sr1 140.5(2) . 3_656 ?
Mo3 Sr4 Sr1 60.80(8) . 3_656 ?
Mo2 Sr4 Sr1 130.02(8) 3_656 3_656 ?
N9 Sr4 Sr7 47.7(3) . . ?
O2 Sr4 Sr7 140.0(3) 3_656 . ?
N1 Sr4 Sr7 87.0(3) . . ?
N6 Sr4 Sr7 128.2(2) 1_556 . ?
N5 Sr4 Sr7 51.4(3) . . ?
O1 Sr4 Sr7 44.43(18) . . ?
Mo3 Sr4 Sr7 65.86(8) . . ?
Mo2 Sr4 Sr7 126.54(7) 3_656 . ?
Sr1 Sr4 Sr7 98.13(7) 3_656 . ?
N9 Sr4 Sr2 127.7(3) . 3_656 ?
O2 Sr4 Sr2 40.7(3) 3_656 3_656 ?
N1 Sr4 Sr2 78.6(3) . 3_656 ?
N6 Sr4 Sr2 46.8(2) 1_556 3_656 ?
N5 Sr4 Sr2 143.5(3) . 3_656 ?
O1 Sr4 Sr2 128.65(18) . 3_656 ?
Mo3 Sr4 Sr2 103.04(9) . 3_656 ?
Mo2 Sr4 Sr2 59.07(7) 3_656 3_656 ?
Sr1 Sr4 Sr2 83.87(8) 3_656 3_656 ?
Sr7 Sr4 Sr2 165.08(5) . 3_656 ?
N9 Sr4 Sr10 102.6(3) . . ?
O2 Sr4 Sr10 152.2(2) 3_656 . ?
N1 Sr4 Sr10 129.0(2) . . ?
N6 Sr4 Sr10 90.1(2) 1_556 . ?
N5 Sr4 Sr10 43.5(2) . . ?
O1 Sr4 Sr10 44.94(18) . . ?
Mo3 Sr4 Sr10 122.75(7) . . ?
Mo2 Sr4 Sr10 70.69(5) 3_656 . ?
Sr1 Sr4 Sr10 134.40(5) 3_656 . ?
Sr7 Sr4 Sr10 57.86(4) . . ?
Sr2 Sr4 Sr10 129.76(6) 3_656 . ?
N1 Sr5 O3 176.4(5) . . ?
N1 Sr5 N7 90.3(4) . 2_757 ?
O3 Sr5 N7 86.9(3) . 2_757 ?
N1 Sr5 N7 90.3(4) . 3_757 ?
O3 Sr5 N7 86.9(3) . 3_757 ?
N7 Sr5 N7 73.2(5) 2_757 3_757 ?
N1 Sr5 N6 92.1(3) . 1_556 ?
O3 Sr5 N6 90.2(3) . 1_556 ?
N7 Sr5 N6 166.4(3) 2_757 1_556 ?
N7 Sr5 N6 93.4(3) 3_757 1_556 ?
N1 Sr5 N6 92.1(3) . 4_566 ?
O3 Sr5 N6 90.2(3) . 4_566 ?
N7 Sr5 N6 93.4(3) 2_757 4_566 ?
N7 Sr5 N6 166.4(3) 3_757 4_566 ?
N6 Sr5 N6 99.9(5) 1_556 4_566 ?
N1 Sr5 Mo1 90.0(3) . 3_757 ?
O3 Sr5 Mo1 86.4(3) . 3_757 ?
N7 Sr5 Mo1 36.6(2) 2_757 3_757 ?
N7 Sr5 Mo1 36.6(2) 3_757 3_757 ?
N6 Sr5 Mo1 130.0(2) 1_556 3_757 ?
N6 Sr5 Mo1 130.0(2) 4_566 3_757 ?
N1 Sr5 Sr2 86.0(3) . 3_656 ?
O3 Sr5 Sr2 97.6(3) . 3_656 ?
N7 Sr5 Sr2 143.2(2) 2_757 3_656 ?
N7 Sr5 Sr2 143.2(2) 3_757 3_656 ?
N6 Sr5 Sr2 50.3(2) 1_556 3_656 ?
N6 Sr5 Sr2 50.3(2) 4_566 3_656 ?
Mo1 Sr5 Sr2 175.98(7) 3_757 3_656 ?
N1 Sr5 Sr8 138.5(2) . 1_556 ?
O3 Sr5 Sr8 44.0(2) . 1_556 ?
N7 Sr5 Sr8 130.3(2) 2_757 1_556 ?
N7 Sr5 Sr8 93.7(3) 3_757 1_556 ?
N6 Sr5 Sr8 46.5(2) 1_556 1_556 ?
N6 Sr5 Sr8 93.3(3) 4_566 1_556 ?
Mo1 Sr5 Sr8 116.59(8) 3_757 1_556 ?
Sr2 Sr5 Sr8 66.80(8) 3_656 1_556 ?
N1 Sr5 Sr8 138.5(2) . 4_566 ?
O3 Sr5 Sr8 44.0(2) . 4_566 ?
N7 Sr5 Sr8 93.7(3) 2_757 4_566 ?
N7 Sr5 Sr8 130.3(2) 3_757 4_566 ?
N6 Sr5 Sr8 93.3(2) 1_556 4_566 ?
N6 Sr5 Sr8 46.5(2) 4_566 4_566 ?
Mo1 Sr5 Sr8 116.59(8) 3_757 4_566 ?
Sr2 Sr5 Sr8 66.80(8) 3_656 4_566 ?
Sr8 Sr5 Sr8 58.38(8) 1_556 4_566 ?
N1 Sr5 Sr6 90.17(5) . 2_656 ?
O3 Sr5 Sr6 89.49(5) . 2_656 ?
N7 Sr5 Sr6 47.9(2) 2_757 2_656 ?
N7 Sr5 Sr6 121.1(2) 3_757 2_656 ?
N6 Sr5 Sr6 145.4(2) 1_556 2_656 ?
N6 Sr5 Sr6 45.6(2) 4_566 2_656 ?
Mo1 Sr5 Sr6 84.46(3) 3_757 2_656 ?
Sr2 Sr5 Sr6 95.54(3) 3_656 2_656 ?
Sr8 Sr5 Sr6 121.77(6) 1_556 2_656 ?
Sr8 Sr5 Sr6 63.61(5) 4_566 2_656 ?
N1 Sr5 Sr6 90.17(5) . 3_656 ?
O3 Sr5 Sr6 89.49(4) . 3_656 ?
N7 Sr5 Sr6 121.1(2) 2_757 3_656 ?
N7 Sr5 Sr6 47.9(2) 3_757 3_656 ?
N6 Sr5 Sr6 45.6(2) 1_556 3_656 ?
N6 Sr5 Sr6 145.4(2) 4_566 3_656 ?
Mo1 Sr5 Sr6 84.46(3) 3_757 3_656 ?
Sr2 Sr5 Sr6 95.54(3) 3_656 3_656 ?
Sr8 Sr5 Sr6 63.61(5) 1_556 3_656 ?
Sr8 Sr5 Sr6 121.77(6) 4_566 3_656 ?
Sr6 Sr5 Sr6 168.92(7) 2_656 3_656 ?
O1 Sr6 N6 95.8(3) 3_656 3_655 ?
O1 Sr6 N3 87.3(3) 3_656 . ?
N6 Sr6 N3 66.8(3) 3_655 . ?
O1 Sr6 N7 87.8(3) 3_656 1_454 ?
N6 Sr6 N7 89.8(3) 3_655 1_454 ?
N3 Sr6 N7 155.5(3) . 1_454 ?
O1 Sr6 N4 176.1(3) 3_656 1_454 ?
N6 Sr6 N4 87.9(3) 3_655 1_454 ?
N3 Sr6 N4 95.2(3) . 1_454 ?
N7 Sr6 N4 91.2(3) 1_454 1_454 ?
O1 Sr6 N7 91.5(3) 3_656 3_656 ?
N6 Sr6 N7 170.7(3) 3_655 3_656 ?
N3 Sr6 N7 108.0(3) . 3_656 ?
N7 Sr6 N7 96.2(3) 1_454 3_656 ?
N4 Sr6 N7 84.9(3) 1_454 3_656 ?
O1 Sr6 Mo2 98.6(2) 3_656 . ?
N6 Sr6 Mo2 34.4(2) 3_655 . ?
N3 Sr6 Mo2 33.7(2) . . ?
N7 Sr6 Mo2 124.1(2) 1_454 . ?
N4 Sr6 Mo2 85.0(2) 1_454 . ?
N7 Sr6 Mo2 138.6(2) 3_656 . ?
O1 Sr6 Sr8 132.7(2) 3_656 . ?
N6 Sr6 Sr8 84.5(3) 3_655 . ?
N3 Sr6 Sr8 49.4(2) . . ?
N7 Sr6 Sr8 139.5(2) 1_454 . ?
N4 Sr6 Sr8 48.6(2) 1_454 . ?
N7 Sr6 Sr8 86.4(2) 3_656 . ?
Mo2 Sr6 Sr8 57.54(7) . . ?
O1 Sr6 Sr10 45.9(2) 3_656 3_656 ?
N6 Sr6 Sr10 93.3(2) 3_655 3_656 ?
N3 Sr6 Sr10 46.0(2) . 3_656 ?
N7 Sr6 Sr10 133.6(2) 1_454 3_656 ?
N4 Sr6 Sr10 135.1(2) 1_454 3_656 ?
N7 Sr6 Sr10 87.7(2) 3_656 3_656 ?
Mo2 Sr6 Sr10 72.02(7) . 3_656 ?
Sr8 Sr6 Sr10 86.88(7) . 3_656 ?
O1 Sr6 Sr3 45.5(2) 3_656 3_656 ?
N6 Sr6 Sr3 141.0(2) 3_655 3_656 ?
N3 Sr6 Sr3 101.4(3) . 3_656 ?
N7 Sr6 Sr3 92.1(2) 1_454 3_656 ?
N4 Sr6 Sr3 130.9(2) 1_454 3_656 ?
N7 Sr6 Sr3 46.1(2) 3_656 3_656 ?
Mo2 Sr6 Sr3 130.59(7) . 3_656 ?
Sr8 Sr6 Sr3 116.92(8) . 3_656 ?
Sr10 Sr6 Sr3 58.59(7) 3_656 3_656 ?
O1 Sr6 Sr9 42.8(2) 3_656 3_656 ?
N6 Sr6 Sr9 94.9(3) 3_655 3_656 ?
N3 Sr6 Sr9 126.3(2) . 3_656 ?
N7 Sr6 Sr9 44.9(2) 1_454 3_656 ?
N4 Sr6 Sr9 135.9(2) 1_454 3_656 ?
N7 Sr6 Sr9 94.4(2) 3_656 3_656 ?
Mo2 Sr6 Sr9 120.06(8) . 3_656 ?
Sr8 Sr6 Sr9 175.49(4) . 3_656 ?
Sr10 Sr6 Sr9 88.70(7) 3_656 3_656 ?
Sr3 Sr6 Sr9 61.16(7) 3_656 3_656 ?
O1 Sr6 Sr3 133.2(2) 3_656 1_454 ?
N6 Sr6 Sr3 90.9(2) 3_655 1_454 ?
N3 Sr6 Sr3 136.8(2) . 1_454 ?
N7 Sr6 Sr3 45.9(2) 1_454 1_454 ?
N4 Sr6 Sr3 45.5(2) 1_454 1_454 ?
N7 Sr6 Sr3 88.2(2) 3_656 1_454 ?
Mo2 Sr6 Sr3 111.88(7) . 1_454 ?
Sr8 Sr6 Sr3 93.99(7) . 1_454 ?
Sr10 Sr6 Sr3 175.81(5) 3_656 1_454 ?
Sr3 Sr6 Sr3 117.53(7) 3_656 1_454 ?
Sr9 Sr6 Sr3 90.48(7) 3_656 1_454 ?
O1 Sr7 O1 180.000(1) 3_756 . ?
O1 Sr7 N9 93.9(4) 3_756 3_756 ?
O1 Sr7 N9 86.1(4) . 3_756 ?
O1 Sr7 N9 86.1(4) 3_756 . ?
O1 Sr7 N9 93.9(4) . . ?
N9 Sr7 N9 180.000(1) 3_756 . ?
O1 Sr7 N5 80.6(3) 3_756 3_756 ?
O1 Sr7 N5 99.4(3) . 3_756 ?
N9 Sr7 N5 72.2(4) 3_756 3_756 ?
N9 Sr7 N5 107.8(4) . 3_756 ?
O1 Sr7 N5 99.4(3) 3_756 . ?
O1 Sr7 N5 80.6(3) . . ?
N9 Sr7 N5 107.8(4) 3_756 . ?
N9 Sr7 N5 72.2(4) . . ?
N5 Sr7 N5 180.0 3_756 . ?
O1 Sr7 Sr9 132.7(2) 3_756 . ?
O1 Sr7 Sr9 47.3(2) . . ?
N9 Sr7 Sr9 99.8(3) 3_756 . ?
N9 Sr7 Sr9 80.2(3) . . ?
N5 Sr7 Sr9 61.6(3) 3_756 . ?
N5 Sr7 Sr9 118.4(3) . . ?
O1 Sr7 Sr9 47.3(2) 3_756 3_756 ?
O1 Sr7 Sr9 132.7(2) . 3_756 ?
N9 Sr7 Sr9 80.2(3) 3_756 3_756 ?
N9 Sr7 Sr9 99.8(3) . 3_756 ?
N5 Sr7 Sr9 118.4(3) 3_756 3_756 ?
N5 Sr7 Sr9 61.6(3) . 3_756 ?
Sr9 Sr7 Sr9 180.0 . 3_756 ?
O1 Sr7 Sr10 48.1(2) 3_756 3_756 ?
O1 Sr7 Sr10 131.9(2) . 3_756 ?
N9 Sr7 Sr10 105.9(3) 3_756 3_756 ?
N9 Sr7 Sr10 74.1(3) . 3_756 ?
N5 Sr7 Sr10 45.7(2) 3_756 3_756 ?
N5 Sr7 Sr10 134.3(2) . 3_756 ?
Sr9 Sr7 Sr10 84.57(7) . 3_756 ?
Sr9 Sr7 Sr10 95.43(7) 3_756 3_756 ?
O1 Sr7 Sr10 131.9(2) 3_756 . ?
O1 Sr7 Sr10 48.1(2) . . ?
N9 Sr7 Sr10 74.1(3) 3_756 . ?
N9 Sr7 Sr10 105.9(3) . . ?
N5 Sr7 Sr10 134.3(2) 3_756 . ?
N5 Sr7 Sr10 45.7(2) . . ?
Sr9 Sr7 Sr10 95.43(7) . . ?
Sr9 Sr7 Sr10 84.57(7) 3_756 . ?
Sr10 Sr7 Sr10 180.0 3_756 . ?
O1 Sr7 Sr4 53.2(2) 3_756 3_756 ?
O1 Sr7 Sr4 126.8(2) . 3_756 ?
N9 Sr7 Sr4 46.2(3) 3_756 3_756 ?
N9 Sr7 Sr4 133.8(3) . 3_756 ?
N5 Sr7 Sr4 51.0(3) 3_756 3_756 ?
N5 Sr7 Sr4 129.0(3) . 3_756 ?
Sr9 Sr7 Sr4 109.97(7) . 3_756 ?
Sr9 Sr7 Sr4 70.03(7) 3_756 3_756 ?
Sr10 Sr7 Sr4 62.78(7) 3_756 3_756 ?
Sr10 Sr7 Sr4 117.22(7) . 3_756 ?
O1 Sr7 Sr4 126.8(2) 3_756 . ?
O1 Sr7 Sr4 53.2(2) . . ?
N9 Sr7 Sr4 133.8(3) 3_756 . ?
N9 Sr7 Sr4 46.2(3) . . ?
N5 Sr7 Sr4 129.0(3) 3_756 . ?
N5 Sr7 Sr4 51.0(3) . . ?
Sr9 Sr7 Sr4 70.03(7) . . ?
Sr9 Sr7 Sr4 109.97(7) 3_756 . ?
Sr10 Sr7 Sr4 117.22(7) 3_756 . ?
Sr10 Sr7 Sr4 62.78(7) . . ?
Sr4 Sr7 Sr4 180.0 3_756 . ?
O3 Sr8 N6 93.2(4) 1_554 . ?
O3 Sr8 N4 164.1(4) 1_554 1_454 ?
N6 Sr8 N4 70.9(4) . 1_454 ?
O3 Sr8 N8 93.8(3) 1_554 3_656 ?
N6 Sr8 N8 98.4(4) . 3_656 ?
N4 Sr8 N8 88.5(3) 1_454 3_656 ?
O3 Sr8 N3 93.3(4) 1_554 . ?
N6 Sr8 N3 157.9(3) . . ?
N4 Sr8 N3 101.6(3) 1_454 . ?
N8 Sr8 N3 102.2(4) 3_656 . ?
O3 Sr8 N4 90.8(3) 1_554 3_756 ?
N6 Sr8 N4 90.3(3) . 3_756 ?
N4 Sr8 N4 89.5(3) 1_454 3_756 ?
N8 Sr8 N4 169.9(4) 3_656 3_756 ?
N3 Sr8 N4 68.4(3) . 3_756 ?
O3 Sr8 Mo2 128.8(3) 1_554 3_655 ?
N6 Sr8 Mo2 35.7(2) . 3_655 ?
N4 Sr8 Mo2 35.3(2) 1_454 3_655 ?
N8 Sr8 Mo2 96.0(3) 3_656 3_655 ?
N3 Sr8 Mo2 132.7(3) . 3_655 ?
N4 Sr8 Mo2 88.1(2) 3_756 3_655 ?
O3 Sr8 Mo2 99.5(3) 1_554 . ?
N6 Sr8 Mo2 123.3(2) . . ?
N4 Sr8 Mo2 89.8(2) 1_454 . ?
N8 Sr8 Mo2 135.0(4) 3_656 . ?
N3 Sr8 Mo2 34.6(3) . . ?
N4 Sr8 Mo2 35.0(2) 3_756 . ?
Mo2 Sr8 Mo2 107.93(8) 3_655 . ?
O3 Sr8 Sr6 142.3(3) 1_554 . ?
N6 Sr8 Sr6 124.4(2) . . ?
N4 Sr8 Sr6 53.6(2) 1_454 . ?
N8 Sr8 Sr6 83.9(3) 3_656 . ?
N3 Sr8 Sr6 51.1(3) . . ?
N4 Sr8 Sr6 86.9(2) 3_756 . ?
Mo2 Sr8 Sr6 88.73(7) 3_655 . ?
Mo2 Sr8 Sr6 59.85(7) . . ?
O3 Sr8 Sr1 46.2(3) 1_554 3_656 ?
N6 Sr8 Sr1 139.2(3) . 3_656 ?
N4 Sr8 Sr1 149.7(2) 1_454 3_656 ?
N8 Sr8 Sr1 89.0(3) 3_656 3_656 ?
N3 Sr8 Sr1 49.7(2) . 3_656 ?
N4 Sr8 Sr1 87.7(2) 3_756 3_656 ?
Mo2 Sr8 Sr1 173.42(6) 3_655 3_656 ?
Mo2 Sr8 Sr1 71.07(8) . 3_656 ?
Sr6 Sr8 Sr1 96.14(8) . 3_656 ?
O3 Sr8 Sr8 45.4(2) 1_554 4_565 ?
N6 Sr8 Sr8 96.0(2) . 4_565 ?
N4 Sr8 Sr8 133.8(2) 1_454 4_565 ?
N8 Sr8 Sr8 48.6(3) 3_656 4_565 ?
N3 Sr8 Sr8 103.6(2) . 4_565 ?
N4 Sr8 Sr8 135.9(2) 3_756 4_565 ?
Mo2 Sr8 Sr8 120.84(4) 3_655 4_565 ?
Mo2 Sr8 Sr8 130.89(5) . 4_565 ?
Sr6 Sr8 Sr8 122.88(5) . 4_565 ?
Sr1 Sr8 Sr8 59.83(4) 3_656 4_565 ?
O3 Sr8 Sr5 46.1(3) 1_554 1_554 ?
N6 Sr8 Sr5 47.3(2) . 1_554 ?
N4 Sr8 Sr5 118.1(2) 1_454 1_554 ?
N8 Sr8 Sr5 95.0(3) 3_656 1_554 ?
N3 Sr8 Sr5 137.1(3) . 1_554 ?
N4 Sr8 Sr5 94.7(2) 3_756 1_554 ?
Mo2 Sr8 Sr5 83.00(7) 3_655 1_554 ?
Mo2 Sr8 Sr5 124.74(8) . 1_554 ?
Sr6 Sr8 Sr5 171.50(5) . 1_554 ?
Sr1 Sr8 Sr5 92.26(8) 3_656 1_554 ?
Sr8 Sr8 Sr5 60.81(4) 4_565 1_554 ?
O1 Sr9 N7 89.5(3) . 3_757 ?
O1 Sr9 N4 89.5(3) . . ?
N7 Sr9 N4 95.1(3) 3_757 . ?
O1 Sr9 N8 156.7(4) . 3_757 ?
N7 Sr9 N8 68.4(4) 3_757 3_757 ?
N4 Sr9 N8 85.5(3) . 3_757 ?
O1 Sr9 N1 89.4(3) . . ?
N7 Sr9 N1 84.4(4) 3_757 . ?
N4 Sr9 N1 178.7(3) . . ?
N8 Sr9 N1 95.4(3) 3_757 . ?
O1 Sr9 N10 115.9(4) . 3_756 ?
N7 Sr9 N10 135.6(4) 3_757 3_756 ?
N4 Sr9 N10 119.3(4) . 3_756 ?
N8 Sr9 N10 86.2(4) 3_757 3_756 ?
N1 Sr9 N10 61.8(4) . 3_756 ?
O1 Sr9 N5 89.0(3) . 3_756 ?
N7 Sr9 N5 156.7(3) 3_757 3_756 ?
N4 Sr9 N5 61.7(3) . 3_756 ?
N8 Sr9 N5 108.3(4) 3_757 3_756 ?
N1 Sr9 N5 118.8(4) . 3_756 ?
N10 Sr9 N5 64.6(4) 3_756 3_756 ?
O1 Sr9 Mo1 124.4(2) . 3_757 ?
N7 Sr9 Mo1 35.1(2) 3_757 3_757 ?
N4 Sr9 Mo1 97.2(2) . 3_757 ?
N8 Sr9 Mo1 34.5(4) 3_757 3_757 ?
N1 Sr9 Mo1 83.0(3) . 3_757 ?
N10 Sr9 Mo1 108.2(3) 3_756 3_757 ?
N5 Sr9 Mo1 141.7(2) 3_756 3_757 ?
O1 Sr9 Mo3 92.3(2) . . ?
N7 Sr9 Mo3 118.1(2) 3_757 . ?
N4 Sr9 Mo3 146.7(2) . . ?
N8 Sr9 Mo3 104.3(2) 3_757 . ?
N1 Sr9 Mo3 33.9(3) . . ?
N10 Sr9 Mo3 33.1(4) 3_756 . ?
N5 Sr9 Mo3 85.1(2) 3_756 . ?
Mo1 Sr9 Mo3 108.89(8) 3_757 . ?
O1 Sr9 Sr7 46.8(2) . . ?
N7 Sr9 Sr7 135.8(2) 3_757 . ?
N4 Sr9 Sr7 91.2(2) . . ?
N8 Sr9 Sr7 155.8(4) 3_757 . ?
N1 Sr9 Sr7 88.4(2) . . ?
N10 Sr9 Sr7 74.6(3) 3_756 . ?
N5 Sr9 Sr7 50.2(2) 3_756 . ?
Mo1 Sr9 Sr7 168.04(5) 3_757 . ?
Mo3 Sr9 Sr7 66.82(7) . . ?
O1 Sr9 Mo2 98.3(2) . 3_756 ?
N7 Sr9 Mo2 126.5(2) 3_757 3_756 ?
N4 Sr9 Mo2 32.8(2) . 3_756 ?
N8 Sr9 Mo2 89.7(4) 3_757 3_756 ?
N1 Sr9 Mo2 148.0(3) . 3_756 ?
N10 Sr9 Mo2 87.2(3) 3_756 3_756 ?
N5 Sr9 Mo2 31.2(2) 3_756 3_756 ?
Mo1 Sr9 Mo2 116.37(8) 3_757 3_756 ?
Mo3 Sr9 Mo2 114.35(8) . 3_756 ?
Sr7 Sr9 Mo2 75.06(7) . 3_756 ?
O1 Sr9 Sr2 143.0(2) . 3_756 ?
N7 Sr9 Sr2 127.4(2) 3_757 3_756 ?
N4 Sr9 Sr2 84.5(2) . 3_756 ?
N8 Sr9 Sr2 59.1(4) 3_757 3_756 ?
N1 Sr9 Sr2 96.7(3) . 3_756 ?
N10 Sr9 Sr2 41.5(4) 3_756 3_756 ?
N5 Sr9 Sr2 56.1(2) 3_756 3_756 ?
Mo1 Sr9 Sr2 92.58(7) 3_757 3_756 ?
Mo3 Sr9 Sr2 74.24(9) . 3_756 ?
Sr7 Sr9 Sr2 96.73(7) . 3_756 ?
Mo2 Sr9 Sr2 59.32(8) 3_756 3_756 ?
N5 Sr10 N2 163.2(5) . . ?
N5 Sr10 O1 84.9(3) . . ?
N2 Sr10 O1 93.5(3) . . ?
N5 Sr10 N3 108.5(4) . 3_656 ?
N2 Sr10 N3 88.1(4) . 3_656 ?
O1 Sr10 N3 86.9(3) . 3_656 ?
N5 Sr10 O2 90.8(4) . . ?
N2 Sr10 O2 94.0(4) . . ?
O1 Sr10 O2 167.3(3) . . ?
N3 Sr10 O2 83.2(4) 3_656 . ?
N5 Sr10 N10 77.4(4) . . ?
N2 Sr10 N10 88.4(4) . . ?
O1 Sr10 N10 116.0(4) . . ?
N3 Sr10 N10 157.0(4) 3_656 . ?
O2 Sr10 N10 74.5(5) . . ?
N5 Sr10 Sr10 123.4(3) . 4 ?
N2 Sr10 Sr10 50.8(2) . 4 ?
O1 Sr10 Sr10 139.74(19) . 4 ?
N3 Sr10 Sr10 106.9(3) 3_656 4 ?
O2 Sr10 Sr10 51.7(2) . 4 ?
N10 Sr10 Sr10 54.6(3) . 4 ?
N5 Sr10 Sr7 53.4(3) . . ?
N2 Sr10 Sr7 114.7(4) . . ?
O1 Sr10 Sr7 45.7(2) . . ?
N3 Sr10 Sr7 125.7(3) 3_656 . ?
O2 Sr10 Sr7 137.8(3) . . ?
N10 Sr10 Sr7 76.1(3) . . ?
Sr10 Sr10 Sr7 126.02(4) 4 . ?
N5 Sr10 Sr2 61.6(3) . . ?
N2 Sr10 Sr2 113.1(2) . . ?
O1 Sr10 Sr2 141.6(2) . . ?
N3 Sr10 Sr2 119.8(3) 3_656 . ?
O2 Sr10 Sr2 42.0(3) . . ?
N10 Sr10 Sr2 42.5(4) . . ?
Sr10 Sr10 Sr2 62.69(4) 4 . ?
Sr7 Sr10 Sr2 96.55(7) . . ?
N5 Sr10 Sr3 116.7(3) . . ?
N2 Sr10 Sr3 53.2(3) . . ?
O1 Sr10 Sr3 47.05(19) . . ?
N3 Sr10 Sr3 106.8(3) 3_656 . ?
O2 Sr10 Sr3 144.1(2) . . ?
N10 Sr10 Sr3 89.0(4) . . ?
Sr10 Sr10 Sr3 92.75(3) 4 . ?
Sr7 Sr10 Sr3 63.37(7) . . ?
Sr2 Sr10 Sr3 131.47(7) . . ?
N5 Sr10 Sr6 112.8(3) . 3_656 ?
N2 Sr10 Sr6 75.6(2) . 3_656 ?
O1 Sr10 Sr6 42.3(2) . 3_656 ?
N3 Sr10 Sr6 49.1(3) 3_656 3_656 ?
O2 Sr10 Sr6 130.7(3) . 3_656 ?
N10 Sr10 Sr6 150.2(4) . 3_656 ?
Sr10 Sr10 Sr6 123.79(4) 4 3_656 ?
Sr7 Sr10 Sr6 87.88(7) . 3_656 ?
Sr2 Sr10 Sr6 167.04(6) . 3_656 ?
Sr3 Sr10 Sr6 61.30(6) . 3_656 ?
N5 Sr10 Sr4 50.2(3) . . ?
N2 Sr10 Sr4 138.2(2) . . ?
O1 Sr10 Sr4 51.1(2) . . ?
N3 Sr10 Sr4 70.8(3) 3_656 . ?
O2 Sr10 Sr4 117.6(2) . . ?
N10 Sr10 Sr4 124.4(3) . . ?
Sr10 Sr10 Sr4 169.20(3) 4 . ?
Sr7 Sr10 Sr4 59.36(6) . . ?
Sr2 Sr10 Sr4 108.76(6) . . ?
Sr3 Sr10 Sr4 98.01(4) . . ?
Sr6 Sr10 Sr4 63.20(5) 3_656 . ?
Mo3 N1 Sr5 177.9(8) . . ?
Mo3 N1 Sr4 88.4(4) . . ?
Sr5 N1 Sr4 92.9(4) . . ?
Mo3 N1 Sr4 88.4(4) . 4_565 ?
Sr5 N1 Sr4 92.9(4) . 4_565 ?
Sr4 N1 Sr4 99.6(5) . 4_565 ?
Mo3 N1 Sr9 88.1(5) . 4_565 ?
Sr5 N1 Sr9 90.3(4) . 4_565 ?
Sr4 N1 Sr9 169.5(5) . 4_565 ?
Sr4 N1 Sr9 90.20(10) 4_565 4_565 ?
Mo3 N1 Sr9 88.1(5) . . ?
Sr5 N1 Sr9 90.3(4) . . ?
Sr4 N1 Sr9 90.20(10) . . ?
Sr4 N1 Sr9 169.5(5) 4_565 . ?
Sr9 N1 Sr9 79.8(4) 4_565 . ?
Mo1 N2 Sr10 135.9(4) . 4 ?
Mo1 N2 Sr10 135.9(4) . . ?
Sr10 N2 Sr10 78.4(4) 4 . ?
Mo1 N2 Sr3 88.9(5) . . ?
Sr10 N2 Sr3 129.4(6) 4 . ?
Sr10 N2 Sr3 81.2(3) . . ?
Mo1 N2 Sr3 88.9(5) . 4 ?
Sr10 N2 Sr3 81.2(3) 4 4 ?
Sr10 N2 Sr3 129.4(6) . 4 ?
Sr3 N2 Sr3 77.2(5) . 4 ?
Mo2 N3 Sr10 132.6(5) . 3_656 ?
Mo2 N3 Sr8 91.0(4) . . ?
Sr10 N3 Sr8 134.2(5) 3_656 . ?
Mo2 N3 Sr1 118.4(5) . 3_656 ?
Sr10 N3 Sr1 87.3(3) 3_656 3_656 ?
Sr8 N3 Sr1 81.2(3) . 3_656 ?
Mo2 N3 Sr6 92.0(4) . . ?
Sr10 N3 Sr6 84.9(4) 3_656 . ?
Sr8 N3 Sr6 79.5(3) . . ?
Sr1 N3 Sr6 144.1(4) 3_656 . ?
Mo2 N4 Sr3 106.7(4) 3_756 . ?
Mo2 N4 Sr8 90.5(4) 3_756 1_656 ?
Sr3 N4 Sr8 162.4(5) . 1_656 ?
Mo2 N4 Sr9 96.6(4) 3_756 . ?
Sr3 N4 Sr9 88.6(3) . . ?
Sr8 N4 Sr9 93.6(3) 1_656 . ?
Mo2 N4 Sr8 87.5(4) 3_756 3_756 ?
Sr3 N4 Sr8 86.2(3) . 3_756 ?
Sr8 N4 Sr8 90.5(3) 1_656 3_756 ?
Sr9 N4 Sr8 174.2(4) . 3_756 ?
Mo2 N4 Sr6 166.9(5) 3_756 1_656 ?
Sr3 N4 Sr6 84.6(3) . 1_656 ?
Sr8 N4 Sr6 77.9(3) 1_656 1_656 ?
Sr9 N4 Sr6 90.1(3) . 1_656 ?
Sr8 N4 Sr6 86.8(3) 3_756 1_656 ?
Mo2 N5 Sr10 150.5(7) . . ?
Mo2 N5 Sr4 105.9(5) . . ?
Sr10 N5 Sr4 86.2(4) . . ?
Mo2 N5 Sr7 127.6(7) . . ?
Sr10 N5 Sr7 80.9(3) . . ?
Sr4 N5 Sr7 77.6(3) . . ?
Mo2 N5 Sr2 82.5(4) . . ?
Sr10 N5 Sr2 74.9(3) . . ?
Sr4 N5 Sr2 151.0(5) . . ?
Sr7 N5 Sr2 119.7(4) . . ?
Mo2 N5 Sr9 81.3(5) . 3_756 ?
Sr10 N5 Sr9 106.7(4) . 3_756 ?
Sr4 N5 Sr9 140.4(5) . 3_756 ?
Sr7 N5 Sr9 68.2(3) . 3_756 ?
Sr2 N5 Sr9 67.5(3) . 3_756 ?
Mo2 N6 Sr8 91.1(4) 3_655 . ?
Mo2 N6 Sr5 176.4(6) 3_655 1_554 ?
Sr8 N6 Sr5 86.2(3) . 1_554 ?
Mo2 N6 Sr6 93.6(4) 3_655 3_655 ?
Sr8 N6 Sr6 94.1(3) . 3_655 ?
Sr5 N6 Sr6 89.0(3) 1_554 3_655 ?
Mo2 N6 Sr2 98.1(4) 3_655 3_655 ?
Sr8 N6 Sr2 93.9(3) . 3_655 ?
Sr5 N6 Sr2 79.7(3) 1_554 3_655 ?
Sr6 N6 Sr2 165.7(5) 3_655 3_655 ?
Mo2 N6 Sr4 92.0(4) 3_655 1_554 ?
Sr8 N6 Sr4 176.0(4) . 1_554 ?
Sr5 N6 Sr4 90.6(3) 1_554 1_554 ?
Sr6 N6 Sr4 88.3(3) 3_655 1_554 ?
Sr2 N6 Sr4 83.1(3) 3_655 1_554 ?
Mo1 N7 Sr9 93.4(5) . 3_757 ?
Mo1 N7 Sr5 88.9(4) . 3_757 ?
Sr9 N7 Sr5 94.8(3) 3_757 3_757 ?
Mo1 N7 Sr3 94.5(4) . . ?
Sr9 N7 Sr3 168.7(5) 3_757 . ?
Sr5 N7 Sr3 93.4(4) 3_757 . ?
Mo1 N7 Sr6 176.6(5) . 1_656 ?
Sr9 N7 Sr6 86.6(3) 3_757 1_656 ?
Sr5 N7 Sr6 87.7(3) 3_757 1_656 ?
Sr3 N7 Sr6 86.0(3) . 1_656 ?
Mo1 N7 Sr6 99.6(4) . 3_656 ?
Sr9 N7 Sr6 89.6(3) 3_757 3_656 ?
Sr5 N7 Sr6 170.2(5) 3_757 3_656 ?
Sr3 N7 Sr6 81.1(3) . 3_656 ?
Sr6 N7 Sr6 83.8(3) 1_656 3_656 ?
Mo1 N8 Sr8 115.4(5) . 2_646 ?
Mo1 N8 Sr8 115.4(5) . 3_656 ?
Sr8 N8 Sr8 82.9(5) 2_646 3_656 ?
Mo1 N8 Sr9 89.1(6) . 3_757 ?
Sr8 N8 Sr9 154.9(7) 2_646 3_757 ?
Sr8 N8 Sr9 91.86(18) 3_656 3_757 ?
Mo1 N8 Sr9 89.1(6) . 2_747 ?
Sr8 N8 Sr9 91.86(18) 2_646 2_747 ?
Sr8 N8 Sr9 154.9(7) 3_656 2_747 ?
Sr9 N8 Sr9 82.6(4) 3_757 2_747 ?
Mo1 N8 Sr2 156.3(8) . 1_556 ?
Sr8 N8 Sr2 81.7(4) 2_646 1_556 ?
Sr8 N8 Sr2 81.7(4) 3_656 1_556 ?
Sr9 N8 Sr2 73.3(3) 3_757 1_556 ?
Sr9 N8 Sr2 73.3(3) 2_747 1_556 ?
Mo3 N9 Sr3 121.3(7) . 3_756 ?
Mo3 N9 Sr4 96.5(5) . . ?
Sr3 N9 Sr4 139.4(6) 3_756 . ?
Mo3 N9 Sr7 112.3(6) . . ?
Sr3 N9 Sr7 91.9(5) 3_756 . ?
Sr4 N9 Sr7 86.2(4) . . ?
Mo3 N9 Sr1 92.4(6) . 3_656 ?
Sr3 N9 Sr1 83.6(4) 3_756 3_656 ?
Sr4 N9 Sr1 80.4(5) . 3_656 ?
Sr7 N9 Sr1 153.1(6) . 3_656 ?
Mo3 N10 Sr2 162.6(12) 3_756 . ?
Mo3 N10 Sr10 108.7(7) 3_756 . ?
Sr2 N10 Sr10 85.3(6) . . ?
Mo3 N10 Sr10 108.7(7) 3_756 4 ?
Sr2 N10 Sr10 85.3(6) . 4 ?
Sr10 N10 Sr10 70.8(5) . 4 ?
Mo3 N10 Sr9 83.8(6) 3_756 3_756 ?
Sr2 N10 Sr9 82.4(5) . 3_756 ?
Sr10 N10 Sr9 105.86(13) . 3_756 ?
Sr10 N10 Sr9 167.6(8) 4 3_756 ?
Mo3 N10 Sr9 83.8(6) 3_756 2_746 ?
Sr2 N10 Sr9 82.4(5) . 2_746 ?
Sr10 N10 Sr9 167.6(8) . 2_746 ?
Sr10 N10 Sr9 105.86(13) 4 2_746 ?
Sr9 N10 Sr9 74.7(5) 3_756 2_746 ?
Sr6 O1 Sr7 173.9(4) 3_656 . ?
Sr6 O1 Sr9 96.1(3) 3_656 . ?
Sr7 O1 Sr9 85.9(3) . . ?
Sr6 O1 Sr10 91.9(3) 3_656 . ?
Sr7 O1 Sr10 86.2(3) . . ?
Sr9 O1 Sr10 172.0(4) . . ?
Sr6 O1 Sr3 92.9(3) 3_656 . ?
Sr7 O1 Sr3 92.7(3) . . ?
Sr9 O1 Sr3 93.4(3) . . ?
Sr10 O1 Sr3 86.3(3) . . ?
Sr6 O1 Sr4 91.7(3) 3_656 . ?
Sr7 O1 Sr4 82.3(2) . . ?
Sr9 O1 Sr4 95.6(3) . . ?
Sr10 O1 Sr4 84.0(3) . . ?
Sr3 O1 Sr4 169.3(3) . . ?
Sr2 O2 Sr1 174.8(7) . . ?
Sr2 O2 Sr10 90.3(4) . . ?
Sr1 O2 Sr10 93.8(4) . . ?
Sr2 O2 Sr10 90.3(4) . 4 ?
Sr1 O2 Sr10 93.8(4) . 4 ?
Sr10 O2 Sr10 76.6(4) . 4 ?
Sr2 O2 Sr4 91.0(4) . 2_646 ?
Sr1 O2 Sr4 85.8(4) . 2_646 ?
Sr10 O2 Sr4 166.6(4) . 2_646 ?
Sr10 O2 Sr4 89.98(10) 4 2_646 ?
Sr2 O2 Sr4 91.0(4) . 3_656 ?
Sr1 O2 Sr4 85.8(4) . 3_656 ?
Sr10 O2 Sr4 89.98(10) . 3_656 ?
Sr10 O2 Sr4 166.6(4) 4 3_656 ?
Sr4 O2 Sr4 103.4(5) 2_646 3_656 ?
Sr8 O3 Sr8 89.3(5) 1_556 4_566 ?
Sr8 O3 Sr1 88.2(4) 1_556 3_657 ?
Sr8 O3 Sr1 88.2(4) 4_566 3_657 ?
Sr8 O3 Sr5 90.0(4) 1_556 . ?
Sr8 O3 Sr5 90.0(4) 4_566 . ?
Sr1 O3 Sr5 177.4(6) 3_657 . ?
Sr8 O3 Sr3 175.4(5) 1_556 2_757 ?
Sr8 O3 Sr3 92.35(10) 4_566 2_757 ?
Sr1 O3 Sr3 87.6(3) 3_657 2_757 ?
Sr5 O3 Sr3 94.3(4) . 2_757 ?
Sr8 O3 Sr3 92.35(10) 1_556 3_757 ?
Sr8 O3 Sr3 175.4(5) 4_566 3_757 ?
Sr1 O3 Sr3 87.6(3) 3_657 3_757 ?
Sr5 O3 Sr3 94.3(4) . 3_757 ?
Sr3 O3 Sr3 85.7(4) 2_757 3_757 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 N2 1.862(14) . ?
Mo1 N8 1.884(18) . ?
Mo1 N7 1.913(11) . ?
Mo1 N7 1.913(11) 4 ?
Mo1 Sr5 3.207(5) 3_757 ?
Mo1 Sr9 3.324(3) 3_757 ?
Mo1 Sr9 3.324(3) 2_747 ?
Mo1 Sr3 3.402(3) . ?
Mo1 Sr3 3.402(3) 4 ?
Mo1 Sr6 3.773(3) 2_646 ?
Mo1 Sr6 3.773(3) 3_656 ?
Mo1 Sr8 3.859(4) 2_646 ?
Mo2 N5 1.818(11) . ?
Mo2 N3 1.871(12) . ?
Mo2 N4 1.891(11) 3_756 ?
Mo2 N6 1.909(11) 3_655 ?
Mo2 Sr8 3.271(3) 3_655 ?
Mo2 Sr8 3.291(3) . ?
Mo2 Sr6 3.372(4) . ?
Mo2 Sr4 3.449(3) 3_656 ?
Mo2 Sr9 3.464(4) 3_756 ?
Mo2 Sr2 3.495(3) . ?
Mo2 Sr3 3.674(3) 3_756 ?
Mo2 Sr4 3.746(3) . ?
Mo3 N9 1.840(13) . ?
Mo3 N9 1.840(13) 4_565 ?
Mo3 N10 1.84(2) 3_756 ?
Mo3 N1 1.870(15) . ?
Mo3 Sr4 3.315(3) . ?
Mo3 Sr4 3.315(3) 4_565 ?
Mo3 Sr9 3.353(3) 4_565 ?
Mo3 Sr9 3.353(3) . ?
Mo3 Sr1 3.444(5) 3_656 ?
Mo3 Sr7 3.730(3) 2_756 ?
Mo3 Sr7 3.730(3) . ?
Mo3 Sr3 3.818(3) 3_756 ?
Sr1 O2 2.394(14) . ?
Sr1 O3 2.525(13) 3_657 ?
Sr1 N3 2.700(12) 3_656 ?
Sr1 N3 2.700(12) 2_646 ?
Sr1 N9 2.835(16) 2_646 ?
Sr1 N9 2.835(16) 3_656 ?
Sr1 Mo3 3.444(5) 3_656 ?
Sr1 Sr4 3.486(3) 2_646 ?
Sr1 Sr4 3.486(3) 3_656 ?
Sr1 Sr8 3.498(3) 3_656 ?
Sr1 Sr8 3.498(3) 2_646 ?
Sr1 Sr3 3.579(4) 4_455 ?
Sr2 O2 2.370(14) . ?
Sr2 N10 2.40(2) . ?
Sr2 N6 2.670(10) 2_645 ?
Sr2 N6 2.670(10) 3_655 ?
Sr2 N8 3.222(17) 1_554 ?
Sr2 N5 3.230(13) . ?
Sr2 N5 3.230(13) 4 ?
Sr2 Sr5 3.414(5) 3_656 ?
Sr2 Mo2 3.495(3) 4 ?
Sr2 Sr10 3.545(3) . ?
Sr2 Sr10 3.545(3) 4 ?
Sr3 N9 2.524(12) 3_756 ?
Sr3 O1 2.611(9) . ?
Sr3 O3 2.643(10) 3_757 ?
Sr3 N4 2.654(10) . ?
Sr3 N7 2.668(11) . ?
Sr3 N2 2.883(14) . ?
Sr3 Sr10 3.559(5) . ?
Sr3 Sr1 3.579(4) 1_655 ?
Sr3 Sr3 3.595(4) 4 ?
Sr3 Sr6 3.658(4) 3_656 ?
Sr3 Mo2 3.674(3) 3_756 ?
Sr4 N9 2.558(15) . ?
Sr4 O2 2.715(9) 3_656 ?
Sr4 N1 2.789(10) . ?
Sr4 N6 2.806(11) 1_556 ?
Sr4 N5 2.816(13) . ?
Sr4 O1 2.859(9) . ?
Sr4 Mo2 3.449(3) 3_656 ?
Sr4 Sr1 3.486(3) 3_656 ?
Sr4 Sr7 3.537(4) . ?
Sr4 Sr2 3.634(3) 3_656 ?
Sr4 Sr10 3.655(3) . ?
Sr5 N1 2.563(15) . ?
Sr5 O3 2.596(13) . ?
Sr5 N7 2.611(11) 2_757 ?
Sr5 N7 2.611(11) 3_757 ?
Sr5 N6 2.656(11) 1_556 ?
Sr5 N6 2.656(11) 4_566 ?
Sr5 Mo1 3.207(5) 3_757 ?
Sr5 Sr2 3.414(5) 3_656 ?
Sr5 Sr8 3.604(3) 1_556 ?
Sr5 Sr8 3.604(3) 4_566 ?
Sr5 Sr6 3.727(3) 2_656 ?
Sr5 Sr6 3.727(3) 3_656 ?
Sr6 O1 2.434(9) 3_656 ?
Sr6 N6 2.663(11) 3_655 ?
Sr6 N3 2.743(12) . ?
Sr6 N7 2.766(11) 1_454 ?
Sr6 N4 2.849(11) 1_454 ?
Sr6 N7 2.949(11) 3_656 ?
Sr6 Sr8 3.462(3) . ?
Sr6 Sr10 3.616(3) 3_656 ?
Sr6 Sr3 3.658(4) 3_656 ?
Sr6 Sr9 3.686(3) 3_656 ?
Sr6 Sr3 3.707(3) 1_454 ?
Sr7 O1 2.498(9) 3_756 ?
Sr7 O1 2.498(9) . ?
Sr7 N9 2.620(15) 3_756 ?
Sr7 N9 2.620(15) . ?
Sr7 N5 2.829(14) 3_756 ?
Sr7 N5 2.829(14) . ?
Sr7 Sr9 3.420(3) . ?
Sr7 Sr9 3.420(3) 3_756 ?
Sr7 Sr10 3.481(3) 3_756 ?
Sr7 Sr10 3.481(3) . ?
Sr7 Sr4 3.537(4) 3_756 ?
Sr8 O3 2.501(10) 1_554 ?
Sr8 N6 2.619(11) . ?
Sr8 N4 2.655(10) 1_454 ?
Sr8 N8 2.656(14) 3_656 ?
Sr8 N3 2.674(11) . ?
Sr8 N4 2.777(10) 3_756 ?
Sr8 Mo2 3.271(3) 3_655 ?
Sr8 Sr1 3.498(3) 3_656 ?
Sr8 Sr8 3.516(4) 4_565 ?
Sr8 Sr5 3.604(3) 1_554 ?
Sr9 O1 2.521(9) . ?
Sr9 N7 2.608(11) 3_757 ?
Sr9 N4 2.694(10) . ?
Sr9 N8 2.769(12) 3_757 ?
Sr9 N1 2.847(12) . ?
Sr9 N10 3.009(18) 3_756 ?
Sr9 N5 3.238(15) 3_756 ?
Sr9 Mo1 3.324(3) 3_757 ?
Sr9 Mo2 3.464(4) 3_756 ?
Sr9 Sr2 3.595(4) 3_756 ?
Sr10 N5 2.524(12) . ?
Sr10 N2 2.574(12) . ?
Sr10 O1 2.596(9) . ?
Sr10 N3 2.610(12) 3_656 ?
Sr10 O2 2.623(11) . ?
Sr10 N10 2.808(18) . ?
Sr10 Sr10 3.253(4) 4 ?
Sr10 Sr6 3.616(3) 3_656 ?
N1 Sr4 2.789(10) 4_565 ?
N1 Sr9 2.847(12) 4_565 ?
N2 Sr10 2.574(12) 4 ?
N2 Sr3 2.883(14) 4 ?
N3 Sr10 2.610(12) 3_656 ?
N3 Sr1 2.700(12) 3_656 ?
N4 Mo2 1.891(11) 3_756 ?
N4 Sr8 2.655(10) 1_656 ?
N4 Sr8 2.777(10) 3_756 ?
N4 Sr6 2.849(11) 1_656 ?
N5 Sr9 3.238(15) 3_756 ?
N6 Mo2 1.909(11) 3_655 ?
N6 Sr5 2.656(11) 1_554 ?
N6 Sr6 2.663(11) 3_655 ?
N6 Sr2 2.670(10) 3_655 ?
N6 Sr4 2.806(11) 1_554 ?
N7 Sr9 2.608(11) 3_757 ?
N7 Sr5 2.611(11) 3_757 ?
N7 Sr6 2.766(11) 1_656 ?
N7 Sr6 2.949(11) 3_656 ?
N8 Sr8 2.656(14) 2_646 ?
N8 Sr8 2.656(14) 3_656 ?
N8 Sr9 2.769(12) 3_757 ?
N8 Sr9 2.769(12) 2_747 ?
N8 Sr2 3.222(17) 1_556 ?
N9 Sr3 2.524(12) 3_756 ?
N9 Sr1 2.835(16) 3_656 ?
N10 Mo3 1.84(2) 3_756 ?
N10 Sr10 2.808(18) 4 ?
N10 Sr9 3.009(18) 3_756 ?
N10 Sr9 3.009(18) 2_746 ?
O1 Sr6 2.434(9) 3_656 ?
O2 Sr10 2.623(11) 4 ?
O2 Sr4 2.715(9) 2_646 ?
O2 Sr4 2.715(9) 3_656 ?
O3 Sr8 2.501(10) 1_556 ?
O3 Sr8 2.501(10) 4_566 ?
O3 Sr1 2.525(13) 3_657 ?
O3 Sr3 2.643(10) 2_757 ?
O3 Sr3 2.643(10) 3_757 ?
